Like this document? Why not share!

# Concrete mix design

## on Feb 25, 2011

• 11,536 views

### Views

Total Views
11,536
Views on SlideShare
11,536
Embed Views
0

Likes
4
327
0

No embeds

### Report content

• Comment goes here.
Are you sure you want to

## Concrete mix designDocument Transcript

• Fundamentals of Concrete Mix Design Table of ContentsINTRODUCTION TO CONCRETE MIX DESIGN…..….…………………………….1TERMINOLOGY ……………………………………………………………………….2ABBREVIATIONS………………………………...……….…………………………..10MIX DESIGN PROCEDURE…………………………………….…………………….11 Course: Concrete FundamentalsInstructor: Dennis Clute, Civil Engineer (Construction); National Design, Construction, and Soil Mechanics Center; Fort Worth, Texas
• Revised March 5, 2003-2-
• INTRODUCTION TO CONCRETE MIX DESIGNSCOPE - This segment of the course is devoted to learning how toproportion select materials that, when properly mixed and properly placed,will produce an economical concrete mix that meets the requirements forplaceability, consistency, strength, durability, and appearance.OBJECTIVE - The objective of this lesson is to learn how to select andproportion the materials for quality concrete.PURPOSE - Our purpose is to develop an understanding of how thecomponents of concrete and the proportioning of those components affectthe end product.GOAL - Our goal is not to simply learn the mechanics of designing aquality concrete mix; it is to obtain the knowledge needed to: • specify the most economical and practical combination of materials, • provide the necessary quality assurance inspection, • analyze and develop solutions to everyday problems that are related to materials and mix proportioning. -3-
• TERMINOLOGYABSORPTION (A) - Absorption is the process by which a liquid is drawn into and tendsto fill permeable pores in a porous solid body. It is expressed as a percentage of the dryweight of the body. For example, the oven dry weight of a sample of sand is 60-poundsand its absorption is 5%. The weight of the sample after it has absorbed all of themoisture it can absorb is: 60 lb x 1.05 = 63 lbsThe amount of water absorbed by the 60-pound sample is: 63 lb - 60 lb = 3 lbsABSOLUTE VOLUME (V) - The absolute volume of a granular material is the volumeof the solid matter in the particles; it does not include the volume of the voids betweenthe particles. The absolute volume of a material is computed as follows: Absolute Volume = weight of material . specific gravity of material x unit weight of waterFor example, the specific gravity of a dry coarse aggregate (Gs) is 2.65. The unit weightof water is 62.4-lb/cu ft. The absolute volume of a 90-lb sample of the aggregate is: Absolute Volume = 90 lb / (2.65 x 62.4 lb/cu ft) = 0.544 cu ft.The absolute volume of a concrete mix can be determined if the weight and bulk specificgravity of the components are known. For a concrete mix with 90-lbs of coarse aggregatewith Gs = 2.65, 60-lbs of fine aggregate with Gs = 2.63, 25-lbs of cement, and 12-lbs ofwater the absolute volume is computed as follows: CA = 90 lb / (2.65 x 62.4 lb/cu ft) = 0.544 cu ft FA = 60 lb / (2.63 x 62.4 lb/cu ft) = 0.366 cu ft Cement = 25 lb / (3.15 x 62.4 lb/cu ft) = 0.127 cu ft Water = 12 lb / (1 x 62.4 lb/cu ft) = 0.192 cu ft Total Volume = 1.229 cu ft.For the same mix containing 4% air the total volume would be: Total Volume = 1.229 cu ft x 1.04 = 1.278 cu ft. -4-
• The volume of air in the mix is: Air = 1.278 cu ft - 1.229 cu ft = 0.049 cu ft.ADD-WATER (AW) - Add-water includes all water and liquid admixtures that areadded to the mix in order to arrive at the amount of free water that is required by the mixdesign. The amount of add-water for a specific mix design changes due to changes in theaggregate moisture.BULK SPECIFIC GRAVITY (Gs) – The bulk specific gravity of a material is the ratioof the weight of a specific absolute volume of the material, excluding the weight of waterwithin the pores, to the weight of an equal volume of distilled water. Simply stated, it isthe unit weight of a dry material (gdry) divided by the unit weight of water (gwater). Gs = gdry / gwater or gdry = Gs x gwaterTo determine the unit weight of a substance like cement, multiply the specific gravity ofthe cement by the unit weight of water. gcement = 3.15 x 62.4 lb/cu ft = 196.56 lb/cu ft Bulk specific gravity of concrete materials Portland Cement 3.15 Pozzolan 2.2 to 2.8 Natural Aggregates 2.4 to 2.9 Water 1.0Bulk specific gravity applies to porous materials. For non-porous materials the specificgravity and bulk specific gravity are the same.BULK SPECIFIC GRAVITY SATURATED SURFACE DRY (Gs(ssd))- The bulkspecific gravity saturated surface dry of a material is the ratio of the weight of a specificabsolute volume of the material, including the weight of water within the pores, to theweight of an equal volume of distilled water. Simply stated, it is the unit weight of asaturated material divided by the unit weight of water and is computed as follows: Gs(ssd) = (1 + Absorption) x Gs(dry).For example, a sample of sand having an absorption of 5% and a specific gravity of 2.63has a bulk specific gravity saturated surface dry that is computed as follows: Gs(ssd) = (1 + 0.05) x 2.63 = 2.76.BULK VOLUME – The volume of a granular material including the volume of the solidparticles and the volume of the voids between the solid particles. -5-
• DRY RODDED UNIT WEIGHT – The dry rodded unit weight of aggregate isdetermined by compacting dry aggregate into a container of a known specific volume asper ASTM test method C 29. The weight of the aggregate is measured and divided by thevolume of the container to yield the dry rodded unit weight in terms of weight per volumesuch as pounds per cubic foot. By knowing the dry rodded unit weight of a nominalmaximum size coarse aggregate and the fineness modulus of the fine aggregate, theweight of the coarse aggregate needed per unit volume of concrete mix can be estimated.FINENESS MODULUS (FM) - The fineness modulus (FM) is a factor obtained byadding the percentages of material in a sample of aggregate that is retained on each of thefollowing sieves: #100, #50, #30, #16, #8, #4, 3/8”, ¾”, 1 ½”, 3”, 6”. The result isdivided by 100 to arrive at the fineness modulus. For conventional concrete the finenessmodulus of the fine aggregate should range from 2.3 to 3.1. A higher fineness modulusrepresents a coarser material and a lower fineness modulus represents a finer material.Knowing the fineness modulus of aggregate gives you some indication of the amount ofpaste needed to make concrete using the aggregate. For instance, sand with a lowfineness modulus has more voids in it and more particle surface, thus, more paste isneeded to fill voids and cement the particles together than would be needed for a coarsersand.Below is an example of the mechanical sieve analysis results of a fine and coarseaggregate with the fineness modulus computed. FINE AGGREGATE COARSE AGGREGATE SIEVE % % % % SIZE PASSING RETAINED PASSING RETAINED 6" 3" 1 1/2" 100 0 3/4" 54.8 45.2 3/8" 100 0 10.4 89.6 #4 97.8 2.2 1.4 98.6 #8 80.1 19.9 0.8 99.2 #16 51.4 48.6 0 100 #30 35.2 64.8 0 100 #50 21.5 78.5 0 100 #100 8.8 91.2 0 100 305.2 732.6 FM = 3.05 FM = 7.33FREE-WATER (FW) – Free-water is the amount of water in the mix that is available tohelp form the paste. (The paste is composed of free-water, cement, pozzolan, andaggregate smaller than the #200 sieve size.) Water that is absorbed by the aggregate isnot free-water. The amount of free-water is shown on the mix design. -6-
• The batch plant operator must ensure that the amount of free-water in the mix does notvary from that called for in the mix design. Batch plant operators monitor aggregatemoisture to determine if there is any free-water in the aggregate or if the aggregate is sodry that it will absorb water that is added to the mix. It is rare to have aggregate at thebatch plant that is in the saturated surface dry condition where the amount of add-waterwould equal the amount of free-water called for in the mix. Batch plant operators have tocompute the amount of add-water by subtracting the amount of aggregate free-water fromthe amount of free-water shown on the mix design. The equation for this is: FWagg = Wagg x (MCagg – Aagg) Add water = free-water shown on the mix design – aggregate free-waterFor example, consider a concrete mix design that calls for 282-pounds of water (i.e. free-water) and contains 1100 pounds of fine aggregate and 2000 pounds of coarse aggregate.The mix design shows fine aggregate absorption to be 2% and coarse aggregateabsorption to be 1%. The batch plant operator measures the aggregate moisture and findsthat the fine aggregate moisture is at 5%. The coarse aggregate, just delivered, has amoisture content of 0.5%. The operator computes the add-water as follows: Fine aggregate = 1100 lbs x (0.05 – 0.02) = + 33 lbs Coarse aggregate = 2000 lbs x (0.005 – 0.01) = - 10 lbs Aggregate free-water + 23 lbs Add-water = water called for in the design - FWagg Add-water = 282 lbs – 23 lbs = 259 lbs.POZZOLAN (p) - A pozzolan is a substance that, in-itself, has little or no cementitiousproperties but when combined with portland cement forms compounds possessingcementitious properties. Fly ash is the most widely used pozzolan.SATURATED SURFACE DRY (SSD) - Saturated surface-dry is the condition of anabsorptive material where the material is saturated but its surface is dry. Saturated surfacedry aggregate neither absorbs water from or contributes water to the concrete mixture.WATER-CEMENT RATIO (w/c) - The water-cement ratio of a concrete mix is theratio of the weight of free-water in the mix to the weight of cement in the mix. It iscomputed on a weight basis by simply dividing the weight of the water in the mix by theweight of the cement in the mix. For example, for a mix containing 282 pounds of waterand 564 pounds of cement the water-cement ratio would be: w/c = 282 lbs / 564 lbs = 0.5WATER-CEMENTITIOUS MATERIALS RATIO (w/(c+p)) - The water-cementitious material ratio is the ratio of the weight of free-water in the mix to the weight -7-
• of cementitious materials in the mix. This term is applicable to a concrete mix thatcontains more than one type of cementitious material as does a mix with cement andpozzolan.WEIGHT (W) - The term weight is commonly used in the construction industry todenote mass. Weight and mass would be the same if gravity were constant. For allpractical purposes, when dealing with concrete components that are weighed in the samegeneral area, the forces due to gravity change so little that weight and mass can be usedinterchangeably. When dealing with concrete components that are weighed atsubstantially different elevations the distinction between mass and weight must be made.In this training course the term weight will be used as if there were no difference betweenweight and mass.VOLUME EQUIVALENCY - Proportioning by the volume equivalency method simplymeans that the volume of cementitious materials (cement + pozzolan) is the same as thevolume of cement in a cement only mix. When proportioning by the volume equivalencymethod w/(c+p) will always be greater than w/c and can be computed by the followingequation: w/(c+p) = 3.15 x w/c , 3.15(1-Fv) + GpFv where Fv = percent fly ash by volume and Gp = specific gravity of the pozzolan.For example, a mix having a water-cement ratio of 0.45 and containing 20 percent fly ashby volume with a specific gravity of 2.3 has a water-cementitious materials ratiocomputed as follows: w/(c+p) = 3.15 x 0.45 = 0.48 3.15(1-0.2) + (2.3 x 0.2)If the percent fly ash in a mix is given based on weight it has a volume equivalency thatis computed by the following equation: Fv = 1 . 1 + (Gp/3.15)((1/Fw)-1)where Fv = percent fly ash by volume, Gp = specific gravity of the pozzolan and Fw =percent fly ash by weight.For example, if a cementitious material is composed of 20% fly ash and 80% cement byweight, and the fly ash specific gravity is 2.3, the percent by volume or volumeequivalency can be computed as follows: Fv = 1 = 0.255 or 25.5% 1 + (2.3/3.15)((1/0.2)-1) -8-
• Percent cement by volume (Cv) = 100 – 25.5 = 74.5%.WEIGHT EQUIVALENCY - Proportioning by the weight equivalency method simplymeans that the weight of cementitious materials (cement + pozzolan) is the same as theweight of cement in a cement only mix. When proportioning by the weight equivalencymethod, if the amount of mix free-water does not change w/c always equals w/(c+p). Ifthe percent fly ash in a mix is given based on volume it can be converted to percent basedon weight by the following equation: Fw = 1 . 1 + (3.15/Gp)((1/Fv)-1)For example, if a cementitious material is composed of 20% fly ash and 80% cement byvolume, and the fly ash specific gravity is 2.3, the percent by weight or weightequivalency can be computed as follows: Fv = 1 = 0.154 or 15.4% 1 + (3.15/2.3)((1/0.2)-1) Percent cement by volume (Cv) = 100 – 15.4 = 84.5%.YIELD, DESIGN YIELD, AND RELATIVE YIELD (Y, Yd, and Ry) – Yield is themeasured volumetric quantity of concrete produced per batch. For example, a trial batchof concrete is batched from the following mix design batching weights: Cement 558 lb Water 204 lb Coarse Aggregate 2016 lb Fine Aggregate 1178 lb Total Weight 3956 lb.After mixing the unit weight is measured to be 145.7 lb/cu ft. The yield is determined asfollows: yield = total weight / unit weight = 3956 lb = 27.15 cu ft. 145.7 lb/cu ftWhen working with inch-pound units the design yield is always 27 cubic feet.Relative yield is the ratio of yield to the design yield. Relative yield = yield / design yield = 27.15 / 27 = 1.006After a trial mix of acceptable consistency, air content, and strength is batched, the trialmix proportions must be adjusted for yield so that the batch plant operator can accurately -9-
• determine the amount of each ingredient needed to produce the exact volume of concretethat is called for. The adjustment is made by multiplying the relative yield by theindividual mix design batching weights as follows: Cement 558 lb x 1.006 = 555 lb/cu yd Water 204 lb x 1.006 = 250 lb/cu yd Coarse Aggregate 2016 lb x 1.006 = 1963 lb/cu yd Fine Aggregate 1178 lb x 1.006 = 1117 lb/cu yd. - 10 -
• ABBREVIATIONSA absorptionABS absoluteabs absorbedAW add-waterc+p cement plus pozzolan or cementitious materialsCA coarse aggregateFA fine aggregateFM fineness modulusFv percent fly ash by volume expressed in decimal formFw percent fly ash by weight expressed in decimal formFW free-waterGp specific gravity of pozzolanGc specific gravity of cementGs bulk specific gravityGs(dry) bulk specific gravity of dry aggregateGs(SSD) bulk specific gravity of saturated surface dry aggregategw unit weight of water (i.e. 62.4 lb/cu. ft.)MC moisture contentOD oven dryP pozzolanRy relative yieldV volumeW weightw/c water-cement ratiow/(c+p) water-cementitious materials ratioY yieldYd design yield (i.e. 27 cu. ft.) - 11 -
• MIX DESIGN PROCEDUREThis segment of the course is devoted to learning how to proportion selectmaterials that, when properly mixed and properly placed, will produce aneconomical concrete mix that meets the requirements for placeability, consistency,strength, durability, and appearance. There are several methods for selecting andadjusting proportions for normal weight concrete. These include: Arbitrary assignment (1:2:3), volumetric Void ratio Fineness modulus Surface area of aggregates Cement content Estimated weight method Absolute volume methodChapter 9 in the Portland Cement Association publication entitled, Design andControl of Concrete Mixes, explains the absolute volume method of proportioningnormal concrete mixtures. This procedure is detailed in the ACI 211.1, StandardPractice for Selecting Proportions for Normal, Heavyweight, and Mass Concreteand has been adopted by the concrete industry as the industry standard procedurefor mix proportioning.The steps in proportioning a mix by the absolute volume method are shown belowwith reference to tables and figures found in Chapter 9 of PCA - Design andControl of Concrete Mixes.1. Determine the required slump from Table 9-6 on page 155.2. Determine the maximum aggregate size based on guidance found on page 152.3. Estimate the quantity of mixing water and air content from Table 9-5 on page 154.4. Select the water-cement ratio based on Tables 9-1, 9-2, and 9-3 on pages 150 and 151.5. Calculate the cement content from the values obtained in steps 3 and 4 above. Reference page 156 for additional guidance.6. Estimate the coarse aggregate content from Table 9-4 on page 152.7. Estimate the fine aggregate content by the absolute volume method by adding the volumes determined in the steps above and subtracting the total from 27.8. Adjust for aggregate moisture as explained on page 164.9. Make trial batch and adjustments as explained on pages 164 and 165. - 12 -
• End of Document - 13 -